# Electronic Structure of a Hydrogenic Acceptor Impurity in Semiconductor Nano-structures

- Shu-Shen Li
^{1, 2}Email author and - Jian-Bai Xia
^{1, 2}

**2**:554

**DOI: **10.1007/s11671-007-9098-9

© to the authors 2007

**Received: **7 September 2007

**Accepted: **21 September 2007

**Published: **9 October 2007

## Abstract

The electronic structure and binding energy of a hydrogenic acceptor impurity in 2, 1, and 0-dimensional semiconductor nano-structures (i.e. quantum well (QW), quantum well wire (QWW), and quantum dot (QD)) are studied in the framework of effective-mass envelope-function theory. The results show that (1) the energy levels monotonically decrease as the quantum confinement sizes increase; (2) the impurity energy levels decrease more slowly for QWWs and QDs as their sizes increase than for QWs; (3) the changes of the acceptor binding energies are very complex as the quantum confinement size increases; (4) the binding energies monotonically decrease as the acceptor moves away from the nano-structures’ center; (5) as the symmetry decreases, the degeneracy is lifted, and the first binding energy level in the QD splits into two branches. Our calculated results are useful for the application of semiconductor nano-structures in electronic and photoelectric devices.

## Introduction

Impurity states play a very important role in the semiconductor revolution. Hydrogenic impurities, including donors and acceptors, have been widely studied in theoretical and experimental approaches [1].

Recently, Mahieu et al. investigated the energy and symmetry of Zn and Be dopant-induced acceptor states in GaAs using cross-sectional scanning tunneling microscopy and spectroscopy at low temperatures [2]. The ground and first excited states were found to have a non-spherical symmetry. In particular, the first excited acceptor state has Td symmetry. Bernevig and Zhang proposed a spin manipulation technique based entirely on electric fields applied to acceptor states in p-type semiconductors with spin-orbit coupling. While interesting on its own, the technique could also be used to implement fault-resilient holonomic quantum computing [3].

Loth et al. studied tunneling transport through the depletion layer under a GaAs surface with a low temperature scanning tunneling microscope. Their findings suggest that the complex band structure causes the observed anisotropies connected with the zinc blende symmetry [4].

Kundrotas et al. investigated the optical transitions in Be-doped GaAs/AlAs multiple quantum wells with various widths and doping levels [5]. The fractional dimensionality model was extended to describe free-electron acceptor (free hole-donor) transitions in a quantum well (QW). The measured photoluminescence spectra from the samples were interpreted within the framework of this model, and acceptor-impurity induced effects in the photoluminescence line shapes from multiple quantum wells of different widths were demonstrated.

Buonocore et al. presented results on the ground-state binding energies for donor and acceptor impurities in a deformed quantum well wire (QWW) [6]. The impurity effective-mass Schrödinger equation was reduced to a one-dimensional equation with an effective potential containing both the Coulomb interaction and the effects of the wire surface irregularities through the boundary conditions. Studying the ground-state wave functions for different positions of the impurity along the wire axis, they found that there are wire deformation geometries for which the impurity wave function is localized either on the wire deformation or on the impurity, or even on both. For simplicity, they only considered hard wall boundary conditions.

Lee et al. calculated the magnetic-field dependence of low-lying spectra of a single-electron magnetic quantum ring and dot, formed by inhomogeneous magnetic fields using the numerical diagonalization scheme [7]. The effects of on-center acceptor and donor impurities were also considered. In the presence of an acceptor impurity, transitions in the orbital angular momentum were found for both the magnetic quantum ring and the magnetic quantum dot when the magnetic field was varied.

Galiev and Polupanov calculated the energy levels and oscillator strengths from the ground state to the odd excited states of an acceptor located at the center of a spherical quantum dot (QD) in the effective mass approximation [8]. They also used an infinite potential barrier model.

Using variational envelope functions, Janiszewski and Suffczynski computed the energy levels and oscillator strengths for transitions between the lowest states of an acceptor located at the center of a spherical QD with a finite potential barrier in the effective mass approximation [9].

Climente et al. calculated the spectrum of a Mn ion in a p-type InAs quantum disk in a magnetic field as a function of the number of holes described by the Luttinger-Kohn Hamiltonian [10]. For simplicity, they placed the acceptor at the center of the disk.

In this paper, we will study the electronic structures and binding energy of a hydrogenic acceptor impurity in semiconductor nano-structures in the framework of effective-mass envelope-function theory. In our calculations, the finite potential barrier and the mixing effects of heavy- and light-holes are all taken into account.

## Theoretical Model

Throughout this paper, the units of length and energy are given in terms of the Bohr radius
and the effective Rydberg constant
where *m*
_{0} and ε_{0} are the mass of a free electron and the permittivity of free space.

In the above equations, γ_{1},γ_{2}, and γ_{3}are the Luttinger parameters and
The subscript *n* = 0, 1, 2,... correspond to the ground-, first excited-, second excited-,... states, respectively. The quantum confinement potential
can be written in different forms for various nano-structures.

*n*-order hydrogenic donor impurity state is explicitly calculated by the following equation:

where *L*
_{
x
}
*L*
_{
y
}, and *L*
_{
z
} are the side lengths of the unit cell in the x, y, and z directions, respectively. *K*
_{
x
} = 2 π /*L*
_{
x
},*K*
_{
y
} = 2 π /*L*
_{
y
},*K*
_{
z
} = 2 π /*L*
_{
z
},*n*
_{
x
} ∈{ − *m*
_{
x
},…, *m*
_{
x
} },*n*
_{
y
} ∈{ − *m*
_{
y
},…, *m*
_{
y
} }, and *n*
_{
z
} ∈{ − *m*
_{
z
},…, *m*
_{
z
}}. The plane wave number is *N*
_{
xyz
} = *N*
_{
x
}
*N*
_{
y
}
*N*
_{
z
} = (2 *m*
_{
x
} + 1)(2 *m*
_{
y
} + 1)(2 *m*
_{
z
} + 1), where *m*
_{
x
}
*m*
_{
y
}, and *m*
_{
z
} are positive integers. We take *L*
_{
x
} = *L*
_{
y
} = *L*
_{
z
} = *L* = *W*
_{max} + 25 nm,*K*
_{
x
} = *K*
_{
y
} = *K*
_{
z
} = *K* = 2 π/*L*, and *N*
_{
x
} = *N*
_{
y
} = *N*
_{
z
} = 7 in the following calculation, where *W*
_{max} is the maximum side length of the nano-structures. If we take larger *N*
_{
x
}
*N*
_{
y
}, and *N*
_{
z
}, the calculation precision will be increased somewhat.

The matrix elements for solving the energy latent root of the impurity states can be found from Eqs. 1 and 5. The electronic structures and binding energy in the nano-structure can be calculated from the matrix elements.

## Results and Discussion

In the following sections, we will give some numerical results for the electronic structure and binding energy of a hydrogenic acceptor impurity in several typical *GaAs*/*Ga*
_{1–x
}
*Al*
_{
x
}
*As* nano-structures. We take the material parameters from Ref. [12]. γ_{1} = 6.98,γ_{2} = 2.06, γ _{3} = 2.93. The band gaps *E*
_{
g
}
^{Γ} (*eV*) of bulk GaAs and *Al*
_{0.35}
*Ga*
_{0.65}
*As* are 1.519 and 2.072 eV, respectively. The valence-band offset is assumed to be 35% of the band gap difference, so *V*
_{0} = 193.55 meV. The dielectric constant ε is taken as 13.1ε_{0}. We adopt a square potential energy model in the following calculation, i.e., *V*(*r*) = 0 inside and *V*(*r*) = *V*
_{0} outside of the nano-structures.

*W*for an acceptor at the QW center. Figure 1 shows that the energy levels monotonically and quickly decrease as the well width increases. It is well known that the donor binding energy has a peak as the QW width increases. However, Fig. 2 shows that the changes of the acceptor binding energies are very complex as the QW width

*W*increases. This is because the holes have asymmetric effective masses, and there are mixing effects between heavy- and light-hole states.

*z*

_{0}for the QW width

*W*= 10

*nm*. This figure shows that the binding energies monotonically decrease as the acceptor moves away from the QW center.

*L*

_{0}(a) and the cylindrical QWW radius (b) for an acceptor at the QWW center. Compared with Fig. 1, we find from Fig. 4 that the impurity energy levels decrease slowly as the QWW size increases. This is because the acceptor is confined in two directions.

*L*

_{0}= 10 nm (a) and for a cylindrical QWW with radius (b). The positions of O, A, and B in Fig. 6a are indicated in the inserted figure. From this figure it is easy see that the binding is the weakest for the impurity located at the corner of the square QWW.

*R*

_{0}(a), the square QD side length

*W*(b), and the cylindrical QD radius and height

*W*( ) (c) for an acceptor at the QD center. Compared with Figs. 1 and 4, we find that the impurity energy levels decrease more slowly in the QD than in the QW or the QWW. This is because the quantum confinement effect is larger in the QD than in the QW and QWW.

*R*

_{0}is greater than about 2.2 nm. The first two quantum states are degenerate and correspond to the first energy level, due to the symmetry of the spherical QD. Figure 8(b) shows that there is only one binding energy level when the side length is between 3 and 10.5 nm. If the side length is greater than 10.3 nm, the second binding energy level arises once again. Figure 8(c) shows that the first two binding energy levels diverge quickly, and the other binding energy levels disappear as the QD radius and height become larger than about 2.5 nm.

*R*

_{0}= 5 nm (a), with a cubic QD side length of

*W*= 10 nm (b), and a cylindrical QD radius and height

*W*equal to 5 nm (c). The impurity positions of O, A, B and C in Fig. 9b and c are indicated on the inserted QD figure, respectively. As the acceptor moves away from the center, the symmetry decreases, the degeneracy is lifted, and the binding energy level splits into two branches. Figure 9c shows that there are two binding energy levels when the cylindrical QD radius and height

*W*equal 5 nm. The binding energy is the largest when the impurity is at the QD center, and it is least when the impurity is at the corner.

## Conclusion

In summary, we have calculated the electronic structures and binding energy levels of a hydrogenic acceptor impurity in 2, 1, and 0-dimensional semiconductor nano-structures in the framework of effective-mass envelope-function theory. Our method can be widely applied in the calculation of the electronic structures and binding energy levels of a hydrogenic acceptor impurity in semiconductor nano-structures of other shapes and other semiconductor material systems. One only needs to specify *V* (**r**) and other material parameters. External field effects are also easily considered with this method.

## Declarations

### Acknowledgments

This work was supported by the National Natural Science Foundation of China under Grant Nos 60325416, 60521001, and 90301007.

## Authors’ Affiliations

## References

- Yoffe AD:
*Adv. Phys.*. 2001,**51:**1. 10.1080/00018730010006608View ArticleGoogle Scholar - Mahieu G, Grandidier B, Deresmes D, Nys JP, Stievenard D, Ebert Ph:
*Phys. Rev. Lett.*. 2005,**94:**026407. COI number [1:CAS:528:DC%2BD2MXmvFSmtA%3D%3D] 10.1103/PhysRevLett.94.026407View ArticleGoogle Scholar - Bernevig BA, Zhang SC:
*Phys. Rev. B*. 2005,**71:**035303. COI number [1:CAS:528:DC%2BD2MXhtVyrtbg%3D] 10.1103/PhysRevB.71.035303View ArticleGoogle Scholar - Loth S, Wenderoth M, Winking L, Ulbrich RG, Malzer S, Dohler GH:
*Phys. Rev. Lett.*. 2006,**96:**066403. COI number [1:CAS:528:DC%2BD28Xhs1Wntbs%3D] 10.1103/PhysRevLett.96.066403View ArticleGoogle Scholar - Kundrotas J, Cerskus A, Asmontas S, Valusis G, Sherliker B, Halsall MP, Steer MJ, Johannessen E, Harrison P:
*Phys. Rev. B*. 2005,**72:**235322. COI number [1:CAS:528:DC%2BD28XlvF2nsg%3D%3D] 10.1103/PhysRevB.72.235322View ArticleGoogle Scholar - Buonocore F, Ninno D, Iadonisi G:
*Phys. Rev. B*. 2000,**62:**10914. COI number [1:CAS:528:DC%2BD3cXnsFWjtb4%3D] 10.1103/PhysRevB.62.10914View ArticleGoogle Scholar - Lee CM, Ruan WY, Li JQ, Lee RCH:
*Phys. Rev. B*. 2005,**71:**195305. COI number [1:CAS:528:DC%2BD2MXlvVOrsrg%3D] 10.1103/PhysRevB.71.195305View ArticleGoogle Scholar - Galiev VI, Polupanov AF:
*Semiconductors*. 1993,**27:**663.Google Scholar - Janiszewski P, Suffczynski M:
*Acta Phys. Pol. A*. 1995,**88:**1171. COI number [1:CAS:528:DyaK28XlsVCm]Google Scholar - Climente JI, Korkusinski M, Hawrylak P, Planelles J:
*Phys. Rev. B*. 2005,**71:**125321. COI number [1:CAS:528:DC%2BD2MXivFensr4%3D] 10.1103/PhysRevB.71.125321View ArticleGoogle Scholar - Cusack MA, Briddon PR, Jaros M:
*Phys. Rev. B*. 1996,**54:**R2300. COI number [1:CAS:528:DyaK28XkslWjsbc%3D] COI number [1:CAS:528:DyaK28XkslWjsbc%3D] 10.1103/PhysRevB.54.R2300View ArticleGoogle Scholar - Vurgaftmana I, Meyer JR:
*J. Appl. Phys.*. 2001,**89:**5815. COI number [1:CAS:528:DC%2BD3MXkt1Wrt74%3D] 10.1063/1.1368156View ArticleGoogle Scholar